Wide band gap thiophosphates ASrPS<sub>4</sub> (A = Li, Na, K, Rb, Cs): cation size effect induced successive structural transformation.
Huang, Yi; Huang, Junben; Zhang, Yong; Dalton transactions (Cambridge, England : 2003) 51 (2022) 15067–15073; doi:10.1039/d2dt02321k

data_7711690
_publ_section_title
;
 Wide band gap thiophosphates ASrPS<sub>4</sub> (A = Li, Na, K, Rb, Cs):
 cation size effect induced successive structural transformation.
;
_journal_issue                   39
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15067
_journal_page_last               15073
_journal_paper_doi               10.1039/d2dt02321k
_journal_volume                  51
_journal_year                    2022
_chemical_formula_moiety         'Cs P S4 Sr'
_chemical_formula_sum            'Cs P S4 Sr'
_chemical_formula_weight         379.74
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_atom_sites_solution_primary     dual
_audit_creation_date             2022-02-23
_audit_creation_method
;
Olex2 1.3
(compiled 2020.06.28 svn.raecde09e for OlexSys, GUI svn.r6132)
;
_audit_update_record
;
2022-04-19 deposited with the CCDC.	2022-09-16 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.0743(12)
_cell_length_b                   6.7904(5)
_cell_length_c                   6.4174(4)
_cell_measurement_reflns_used    2756
_cell_measurement_temperature    293.0
_cell_measurement_theta_max      27.32
_cell_measurement_theta_min      3.75
_cell_volume                     787.62(9)
_computing_cell_refinement       'SAINT V8.38A (Bruker, 2018)'
_computing_data_reduction        'SAINT V8.38A (Bruker, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      293.0
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0990
_diffrn_reflns_av_unetI/netI     0.0396
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            10918
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.513
_diffrn_reflns_theta_min         2.254
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    12.553
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5585
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            'clear dark colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.202
_exptl_crystal_description       block
_exptl_crystal_F_000             688
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.102
_refine_diff_density_max         1.287
_refine_diff_density_min         -1.069
_refine_diff_density_rms         0.178
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.138
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         985
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.138
_refine_ls_R_factor_all          0.0382
_refine_ls_R_factor_gt           0.0313
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0231P)^2^+3.2539P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0750
_refine_ls_wR_factor_ref         0.0797
_reflns_Friedel_coverage         0.000
_reflns_number_gt                853
_reflns_number_total             985
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d2dt02321k2.cif
_cod_data_source_block           CsSrPS4
_cod_database_code               7711690
_shelx_shelxl_version_number     2018/3
_olex2_refinement_description
;
;
_shelx_res_checksum              99681
_olex2_submission_special_instructions 'No special instructions were received'